| ||Format||Pages||Price|| |
|17||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||17||$52.00||  ADD TO CART|
Significance and Use
5.1 Solar-energy absorptance, reflectance, and transmittance are important in the performance of all solar energy systems ranging from passive building systems to central receiver power systems. This test method provides a means for determining these values under fixed conditions that represent an average that would be encountered during use of a system in the temperate zone.
5.2 Solar-energy absorptance, reflectance, and transmittance are important for thermal control of spacecraft and the solar power of extraterrestrial systems. This test method also provides a means for determining these values for extraterrestrial conditions.
5.3 This test method is designed to provide reproducible data appropriate for comparison of results among laboratories or at different times by the same laboratory and for comparison of data obtained on different materials.
5.4 This test method has been found practical for smooth materials having both specular and diffuse optical properties. Materials that are textured, inhomogeneous, patterned, or corrugated require special consideration.
5.4.1 Surface roughness may be introduced by physical or chemical processes, such as pressing, rolling, etching, or deposition of films or chemical layers on materials, resulting in textured surfaces.
5.4.2 The magnitude of surface roughness with respect to the components of the spectrophotometer and attachments (light beam sizes, sphere apertures, sample holder configuration) can significantly affect the accuracy of measurements using this test method.
5.4.3 Even if the repeatability, or precision of the measurement of textured materials is good, including repeated measurements at various locations within or orientations of the sample, the different characteristics of different spectrophotometers in different laboratories may result in significant differences in measurement results.
5.4.4 In the context of 5.4.3, the term ‘significant’ means differences exceeding the calibration or measurement uncertainty, or both, established for the spectrophotometers involved, through measurement of or calibration with standard reference materials.
5.5 This test method describes measurements accomplished over wider spectral ranges than the Photopic response of the human eye. Measurements are typically made indoors using light sources other than natural sunlight, though it is possible to configure systems using natural sunlight as the illumination source, as in Practice E424. Practice E971 describes outdoor methods using natural sunlight over the spectral response range of the human eye.
5.6 Light diffracted by gratings is typically significantly polarized. For polarizing samples, measurement data will be a function of the orientation of the sample. Polarization effects may be detected by measuring the sample with rotation at various angles about the normal to the samples.
1.5 Transmitting sheet materials that are inhomogeneous, textured, patterned, or corrugated require special considerations with respect to the applicability of this test method. Test Method E1084 may be more appropriate to determine the bulk optical properties of textured or inhomogeneous materials.
1.6 For homogeneous materials this test method is preferred over Test Method E1084.
1.7 This test method refers to applications using standard reference solar spectral distributions but may be applied using alternative selected spectra as long as the source and details of the solar spectral distribution and weighting are reported.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E275 Practice for Describing and Measuring Performance of Ultraviolet and Visible Spectrophotometers
E424 Test Methods for Solar Energy Transmittance and Reflectance (Terrestrial) of Sheet Materials
E490 Standard Solar Constant and Zero Air Mass Solar Spectral Irradiance Tables
E772 Terminology of Solar Energy Conversion
E971 Practice for Calculation of Photometric Transmittance and Reflectance of Materials to Solar Radiation
E1084 Test Method for Solar Transmittance (Terrestrial) of Sheet Materials Using Sunlight
E1175 Test Method for Determining Solar or Photopic Reflectance, Transmittance, and Absorptance of Materials Using a Large Diameter Integrating Sphere
E2554 Practice for Estimating and Monitoring the Uncertainty of Test Results of a Test Method in a Single Laboratory Using a Control Sample Program
G173 Tables for Reference Solar Spectral Irradiances: Direct Normal and Hemispherical on 37 Tilted Surface
G197 Table for Reference Solar Spectral Distributions: Direct and Diffuse on 20 Tilted and Vertical Surfaces
Other DocumentsNIST SP 250-69 Regular Spectral Transmittance Available on line at http://www.nist.gov/calibrations/upload/SP250-69.pdf
ICS Number Code 77.140.80 (Iron and steel castings)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E903-12, Standard Test Method for Solar Absorptance, Reflectance, and Transmittance of Materials Using Integrating Spheres, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top